To cite this version:
Maxime l’Héritier, Sandrine Baron, Laurent Cassayre, Florian Téreygeol. Bismuth behaviour during ancient processes of silver–lead production. Journal of Archaeological Science, Elsevier, 2015, 57, pp.56-68. 10.1016/j.jas.2015.02.002. hal-01187779
HAL Id: hal-01187779 https://hal.archives-ouvertes.fr/hal-01187779 Submitted on 9 Nov 2018
HAL is a multi-disciplinary open access L’archive ouverte pluridisciplinaire HAL, est archive for the deposit and dissemination of sci- destinée au dépôt et à la diffusion de documents entific research documents, whether they are pub- scientifiques de niveau recherche, publiés ou non, lished or not. The documents may come from émanant des établissements d’enseignement et de teaching and research institutions in France or recherche français ou étrangers, des laboratoires abroad, or from public or private research centers. publics ou privés. OATAO is an open access repository that collects the work of Toulouse researchers and makes it freely available over the web where possible
This is an author’s version published in: http://oatao.univ-toulouse.fr/20598
Official URL: https://doi.org/10.1016/j.jas.2015.02.002
To cite this version: L'Héritier, Maxime and Baron, Sandrine and Cassayre, Laurent and Téreygeol, Florian Bismuth behaviour during ancient processes of silver–lead production. (2015) Journal of Archaeological Science, 57. 56-68. ISSN 0305-4403
Any correspondence concerning this service should be sent to the repository administrator: [email protected] Bismuth behaviour during ancient processes of silverelead production
* Maxime L'Heritier a, , Sandrine Baron b, c, Laurent Cassayre d, e, Florian Tereygeol f a Universite Paris 8, EA 1571, Centre de Recherches Historiques: Histoire des Pouvoirs, Savoirs et Societes, 2 rue de la Liberte, 93526 Saint-Denis Cedex, France b Universite de Toulouse Jean-Jaures, Laboratoire TRACES, Maison de la Recherche, 5 allees Antonio-Machado, F-31 058 Toulouse Cedex 09, France c CNRS, Laboratoire des Travaux et Recherches Archeologiques sur les Cultures, les Espaces et les Societes, F-31058 Toulouse, France d Universite de Toulouse, INP, UPS, Laboratoire de Genie Chimique, 4 Allee Emile Monso, F-31030 Toulouse, France e CNRS, Laboratoire de Genie Chimique, F-31030 Toulouse, France f Institut de Recherches sur les Archeomateriaux (IRAMAT), CNRS UMR 5060, LMC e LAPA, Bat 637 CEA e Saclay, 91191 Gif-sur-Yvette Cedex, France article info a b s t r a c t
Keywords: Bismuth is one of the main trace elements found in archaeological lead and silver material in very Cupellation variable contents. As silver reﬁning by cupellation involves the redistribution of some trace elements Fire-assay contained in the initial lead bullion into the litharge and silver phases, an interdisciplinary approach has Thermodynamics been carried out to understand the behaviour of bismuth during this process. Twenty-eight ﬁre-assays Experimental archaeology were processed with seven different PbeBieAg alloys of various Bi content. A chemical characterization Trace elements of all products was carried out. Parallel to the experiments, a thermodynamic approach was undertaken. Silver The combination of experiments and modelling shows that the Bi/Pb ratio can be used as a tracer in silver Lead material throughout the whole cupellation process. Bi and Ag contents in metallic lead might as well highlight the metallurgical process used to obtain lead. High Bi contents in silverelead bullions are shown to notably reduce the silver extraction yield.
1. Introduction in Egyptian net sinkers (Rehren and Prange, 1998) and in diverse material coming from ancient Thrace and from the Black Sea (Kuleff The present work places speciﬁc attention on the behaviour of et al., 1995, 2006). Kuleff et al. (2006) even report a lead anchor bismuth (Bi) in ancient processes of silverelead production. Bi from the Euxine exceeding 2 wt.% Bi. However, most archaeological content is extremely variable in both lead and silver archaeological lead artefacts are below 100 ppm and very often below 10e20 ppm artefacts reported in literature. Regarding silver material, most Bi, e.g. medieval and modern stained-glass joints dated from the Carolingian deniers (silver coins) contain a few hundreds ppm Bi 8th to the 17th centuries (Cuzange and Texier, 2000). Among 40 (Sarah et al., 2008; Sarah, 2012). Yet, some authors also cite oriental lead objects from Nuragic Sardinia more than a third have less than silver coins containing up to several percent of Bi (Mac Kerrel and 1 ppm Bi, the maximum recorded being 80 ppm (Atzeni et al., 2003; Stevenson, 1972; Cowell and Lowick, 1988). Sarah (2012) reports Cincotti et al., 2003). The Bi content of Hellenistic lead ingots, as well silver dirhams with up to 0.6 wt.% Bi. Likewise in prehistoric sheets and trephines are scattered between 30 and 45 ppm and ancient Spain, data summed up by Hunt Ortiz (2003) show that (Asderaki and Rehren, 2006). For lead objects excavated in Rhine- Bi content in silver is usually low (<0.1 wt.%), yet a sample of un- land and Westphalia from AugustaneTiberian military camps reﬁned silver (91 wt.%) from Rio Tinto dated from the Roman period (Bode, 2008) it is usually lower than the detection limit of their and analysed by Craddock et al. (1985) bears as much as 4.6 wt.% Bi. analytic procedure (10 ppm). All Roman lead ingots analysed by Regarding lead artefacts, very high Bi concentrations ranging Baron and Cochet (2003) are likewise below 10 ppm Bi. Eventually, from several hundred ppm up to a few thousand ppm are observed despite some very rich artefacts, most objects reported by Kuleff et al. (1995, 2006) have a very low Bi content (<20 ppm). These compositions offer a stunning paradox with the known characteristics of contemporary lead metallurgy: at the present day, * Corresponding author. bismuth extraction from the lead bullion is a real challenge with E-mail address: [email protected] (M. L'Heritier). http://dx.doi.org/10.1016/j.jas.2015.02.002 standard reﬁning techniques, such as pyrolysis or electroreﬁning L'Heritier and Tereygeol (2010) state that Bi content is ten to thirty (Ramachandra Rao, 2006). As the presence of Bi lowers mechanical times lower in lead resmelted from litharge collected during properties and corrosion resistance of Pb based alloys, bismuth cupellation than in the initial leadesilver bullion. There is however puriﬁcation is a crucial operation in many domains, which actually no further interpretation of Bi content in ancient artefacts: this became one of the metallurgical challenges during the 20th cen- point has never been fully discussed and Bi is usually only tury. Several treatments (basically by the addition of alkaline ele- considered as an ore source tracer (Cuzange and Texier, 2000; ments or antimony) were developed to reduce Bi content in lead Baron and Cochet, 2003; Kuleff et al., 2006; Forel et al., 2010) materials down to 60 ppm on average (Kroll, 1922; Betterton and despite all issues linked to ore or metal mixing and remelting (e.g. Lebedeff, 1936; Kroll, 1938; Evers, 1949; Defonte, 1964) and Anguilano et al., 2010). Thus, there is a need to estimate the impact improved to reach the level of 10 ppm Bi in lead bullion (Ng and of the cupellation process on the impurities dispersion between Siviour, 1994; Lu et al., 2011), which is common in most archaeo- lead and silver button as well as the role of the ores elemental logical materials. However, before the identiﬁcation of the element composition. Bi by French and German chemists Claude Geoffroy the Younger The question eventually comes down to: Is Bi a tracer for and J. H. Pott in the mid 17th century (Pott, 1738; Grandjean de metallurgical process rather than a tracer for ores sources? And Fouchy 1757), debismuthizing according to the above-mentioned how are technological choices and archaeological remains processes could certainly not be used by ancient metallurgists. impacted by the treatment of such Bi rich ores? These crucial his- Ancient lead production processes must therefore be investigated torical questions are also linked to the use of lead ores and the trade to shed light on such compositions. of unreﬁned lead produced in certain European countries where Lead was then mostly a by-product of silver production. On the leadesilver production was important. It was therefore necessary one hand, galena, i.e. lead sulphide, was among the main silver ores to focus on understanding Bi behaviour during the cupellation processed before the modern times. On the other hand, high process. For this purpose, the approach included: amounts of lead were also required to retrieve silver from any polymetallic ore e e.g. jarosite in Rio Tinto (Anguilano et al., 2010) e Fire-assaying (i.e. cupellation) of “home-made” lead ingots and, in particular, from low grade copper ores with the liquation processed on the international site dedicated to experimental and drying process which was developed in the end of the Middle paleometallurgy in Melle (France), according to the ﬂowchart Ages (Suhling, 1976, 1994; L'Heritier et al., 2010). Details about the presented in Fig. 1. The Bi content of the ingots ranged from ancient leadesilver chaîne operatoire are reported elsewhere 130 ppm to 78 000 ppm: some of these materials were notably (Tylecote, 1976; Baron et al., 2009). Lead and silver were then much richer in Bi than most archaeological ores, since the pur- separated via the cupellation process, used in ancient and medieval pose was to verify the potential effect of Bi on the cupellation times to retrieve silver from argentiferous lead ingots (Tylecote, process. 1976; Tereygeol and Thomas, 2003). This process involves the Chemical characterisation of all products i.e. “home-made” oxidation of the silver-containing lead bullion in air at a tempera- initial alloys, cupels impregnated with litharge and silver ture of about 900e950 C, producing silver metal and lead oxide buttons. (also called litharge) as separate phases. The trace elements con- A modelling of the chemical equilibrium involved in the tained in the initial lead bullion are separated according to their cupellation process, using computational thermodynamics and afﬁnity with oxygen: noble elements tend to stay in the silver modern data. This approach was driven by a model aiming at button, whereas elements which oxidise end up in litharge and sharpening the prediction of process performances proposed by therefore in the resulting metallic lead obtained after litharge Swinbourne et al. (2003), in the frame of the improvement of resmelting (Tereygeol and Thomas, 2003). The impact of the the modern industrial cupellation technology. cupellation process on the chemical repartition of trace elements and speciﬁcally Bi should thus be questioned. Discussions regarding Bi behaviour during silver reﬁning have 2. Materials and methods been contradictory. In the 19th century, elemental Bi was consid- ered as strongly volatile by French assayer Chaudet (1818) and 2.1. Pb based alloys preparation mining engineer Berthier (1834), later endorsed by Matthey (1887). Berthier (1834) also registered a higher silver loss when using In order to evaluate the inﬂuence of the initial Bi content on the bismuth instead of lead for cupellation. Metallurgical treatises from behaviour of the other elements and on the cupellation products, the end of the 19th century claim on the other hand that Bi, like two experimental cupellation campaigns (XP1 and XP2) were car- noble metals, has a small afﬁnity for oxygen and therefore stays ried out, using as starting material PbeBieAgeSbeSn alloys of concentrated in the metal phase (Percy, 1870; Schnabel, 1898). various compositions. Overall, seven different Pb based alloys were Taking the example of Bi-rich litharge derived from lead ores of the prepared, with constant (1 wt.%) Ag content (representative of Upper Harz, Percy (1870) even adds that Bi oxidises at the end of silver-rich lead bullions, e.g. obtained from galena smelting) and Bi the operation, just shortly before the “blick” i.e. with the last contents ranging from 130 ppm to 78 000 ppm. All alloys were litharge. This last theory was endorsed in the 20th century by prepared using pure silver powder (Goodfellow AG006021/2 at several works (Shepard and Dietrich, 1940; Pernicka and 99.99%) and bismuth (>99% as analysed by portable XRF Thermo Bachmann, 1983; Raub, 1995). Yet, if the general behaviour of bis- Scientiﬁc Niton Xl3t). The lead source was slightly different be- muth during cupellation is by no means controversial anymore, the tween the two campaigns. As evidenced in Table 1, which sum- precise conditions of bismuth partitioning between lead oxide and marizes the composition of each Pb based alloy, the ingots used in silver and its inﬂuence on cupellation products remain largely XP1 present higher Sb and Sn content than ingots used in XP2. understudied. Experiments carried out by Pernicka and Bachmann These “home-made” ingots can be considered as archaeological (1983) show that bismuth oxidizes after lead. According to them, lead analogues with different impurities reﬂecting the lead pro- when 99.9% of the lead has already oxidised, 50% of the bismuth is duction of different mining districts. still present in the silver bead. Yet, they give no interpretation about As the Pb based alloys melt at ca. 300 C, they were prepared in a the inﬂuence of the initial Bi content on the silver yield nor on the laboratory furnace at 450 C. First, lead was heated in a lidded lead and silver materials produced. Regarding this last point, graphite crucible for 30 min. Then, silver and bismuth were added, Fig. 1. Flowchart of the experimental cupellation process and experimental furnace used during the experiments. and the bath was stirred with a small wooden spatula before ﬁnal Bone ash cupels are considered as inert material which does not homogenisation for 30 min in the furnace. Eventually, the alloys react with litharge. In ancient times, however, textbooks as well as were cast in ingots in a sand casting mould. 100 g of each alloy were archaeological remains testify that, if the usual preference was prepared, which allowed performing four assays of approx. 20 g per indeed for bone ash, many other recipes were used depending on batch. All Pb based alloys were characterised using ICP-MS (HR-ICP- metallurgical traditions or more simply due to the availability of MS) equipment by ALS laboratory. Table 1 Composition of the processed Pb based alloys. The chemical characterisation was 2.2. Cupels composition performed using ICP-SMS (HR-ICP-MS) by ALS laboratory.
Reference Pb (wt.%) Ag (ppm) Bi (ppm) Sb (ppm) Sn (ppm) Cupels used for the present study are industrial bone ash cupels, with an inverted truncated cone shape and a weight of about 65 g. XP1.1 94.9 7300 130 42 000 660 XP1.2 93.8 10 000 3000 42 000 6700 Their dimensions are as follows: external diameter is 5 cm on top XP1.3 88.9 10 000 21 000 72 000 6500 and 4 cm at the bottom, height is 2.5 cm and the cavity has a XP2.1 98.0 10 100 9900 3.8 1.5 diameter of 3.5 cm and is ~1 cm deep in the middle. A preliminary XP2.2 97.0 10 200 19 400 10.5 3.4 chemical characterisation of the cupels indicated no metal XP2.3 95.1 10 000 38 600 8.3 2.7 XP2.4 91.1 10 200 78 100 3.0 2.1 contamination. materials: wood ash, bone ash, a mixture of the two or even clay involved during the cupellation process. For this purpose, the hearths topped with a non-siliceous lining (Agricola, 1556; Bayley Equilibrium Module of the FactSage™ software (Bale et al., 2002) and Eckstein, 2006; Biringuccio, 1540; Ercker, 1580; Hawthorne was used, taking into account the multicomponent system (Pb, Ag, and Smith, 1979; Martinon-Torres et al., 2008, 2009). All these Bi, Sb, Sn, O2,N2) and three major phases: a liquid metal phase (i.e. materials may behave slightly differently during cupellation, and the lead bullion converted into a silver button), a liquid oxide phase the formation of lead silicates or calciumesilicaephosphates is (i.e. the PbO based litharge) and a gas phase (i.e. air). likely to diminish their capacity to absorb metallic oxides (Bayley The SGTE (Scientiﬁc Group Thermodata Europe, www.stge.org) and Eckstein, 2006; Rehren, 1998). Martinon-Torres et al. (2008, Solution database was used to model the liquid metal phase, while 2009) however proved that whenever a top layer of bone ash is air (a mixture of 20 mol.% O2 and 80 mol.% N2) was modelled with used, the separation of silver is just as easy as with an entirely bone the SGTE Pure Substances database. No database was available for ash cupel. These former studies on cupellation materials also the liquid oxide phase, it was thus modelled as an ideal PbO liquid showed that the composition of cupellation hearth has a negligible phase containing dilute amounts of AgO0.5, SnO2, SbO1.5 and BiO1.5, inﬂuence on the composition of the litharge cakes produced and on using speciﬁc Henrian activity coefﬁcients for each compound. subsequent silver losses (Bayley and Eckstein, 2006). Activity coefﬁcients were assessed based on literature data from Ueda (2005, 2009). The selected activity coefﬁcients are compiled 2.3. Fire-assay of the Pb based alloys in Table 2. With these parameters, the following major properties of the systems are well reproduced at 1000 C: Ag solubility of about Fire assaying was performed in a replica of ﬁre-assay furnaces 5 wt.% both in PbO (Shao et al., 1993) and in Bi2O3 (Assal et al., 1999) depicted by Agricola, 1556. The internal diameter of the furnace is in air, full miscibility of Bi2O3 and PbO (Diop et al., 2009), distri- 26 cm and the mufﬂe in which the cupels were placed is 24 cm long, bution ratio of Ag in PbePbO (Ueda et al., 2005), distributions ratio 13 cm wide and 9 cm in height. During the two campaigns, the of Sn, Sb and Bi between AgePb alloy and PbO (Ueda et al., 2009). assays were carried out one after another, in similar conditions, Given that, after preliminary calculations, Sn and Sb elements starting with the lowest Bi concentrations to prevent any pollution. were found as the main elements to oxidise at the very beginning of The mufﬂe temperature was monitored with a thermocouple. Prior cupellation, an additional ideal SnO2eSb2O3 solid solution to the start of experimental campaigns, the furnace was preheated described by Zaharescu (Zaharescu et al., 1991) was taken into ac- for 150 min, until an adequate temperature was reached (~900 C). count, while the liquid phase was considered as an ideal Each ﬁre-assay was then performed as follows: a fresh cupel con- Sb2O3ePbO mixture (Kopyto et al., 2009). taining the lead bullion was positioned in the centre of the mufﬂe In order to model the cupellation process, calculations were and the furnace door was closed until temperature stabilised and performed as follows: the alloy was melted. Then, the furnace door was slightly opened to let air in. Regular charcoal supply helped controlling the tempera- (i) the initial system was the lead bullion (100 g) at 1000 C, ture inside the furnace: the thermocouple placed right above the (ii) a given amount of air (typically 1.25 mol, i.e. about 3.7 dm3) cupel indicated a variation from 850 to 980 C during the entire was added in the system and the equilibrium was computed, session. Finally, after the “blick”, the cupel was withdrawn and the (iii) litharge, formed by reaction of the alloy with air, was next one placed inside the furnace. Each run lasted between 30 and removed from the system, in order to represent its ﬂow into 40 min and produced a silver button. Apart from the ﬁrst ﬁre-assay, the cupel, escaping of the entrapped gases during cooling created cauli- (iv) steps (ii) and (iii) were repeated with the remaining metal ﬂowering aspect on the surface of the button. phase until the oxidation reaction was completed.
2.4. Chemical characterisation of litharge impregnated cupels and Litharge and metal compositions were stored after each calcu- silver buttons lation step, in order to follow the evolution of composition of both phases during cupellation. Preliminary calculations using as Litharge impregnated cupels were analysed by SEM-EDS benchmark the modelling of a modern industrial cupellation pro- (scanning electron microscopy-energy dispersive spectroscopy) cess, published by Swinbourne et al. (2003), gave satisfactory re- and microprobe. Elemental analyses were carried out for one cupel sults regarding Ag recovery yield and ﬁnal Pb content in the silver of each assay of XP 1, and concentration proﬁles through the cupels product. as well as elemental mappings were obtained. The silver buttons In order to compare the calculations involving initial lead bul- were analysed by LA-ICP-MS (laser ablation inductively coupled lions of various AgeBieSbeSn contents, a so-called “cupellation plasma mass spectrometry) according to a protocol published progress”, calculated as the amount (in mol) of O2 added at a given elsewhere (Sarah et al., 2007). Reference materials whose compo- step divided by the total O2 addition, was chosen to represent the sitions are close to the silver buttons (i.e. silver alloys containing up to 15 wt.% Cu doped with up to 2 wt.% Zn, Sn, Au, Pb and Bi) were Table 2 used for normalisation. The composition of each silver sample was Input data for the model of the PbO based slag phase in the Equilibrium Module of determined by calculating mean values on the homogeneous FactSage™. fraction of the signal. Compound (SGTE pure Reference Form in New log (g) at References An inter comparison between LA-ICP-MS and HR-ICP-MS substance database) state PbO slag mixing 1000 C analytical techniques was carried out on some lead and silver particle materials: the calculated analytical difference was less than 10% for PbO liq e e e e all trace elements considered (Ag, Bi, Sn, Sb), which is on the same Ag2O s AgO0.5 2 À0.65 Ueda et al., range as the intrinsic error of each analytical method. 2005 Bi2O3 liq BiO1.5 2 À0.70 Ueda et al., 2009
2.5. Thermodynamic modelling of cupellation Sb2O3 liq SbO1.5 2 0.46 Ueda et al., 2009 Parallel to the experiments, a computational thermodynamics SnO2 liq SnO2 1 1.50 Ueda et al., 2009 study was undertaken in order to model the chemical equilibriums reaction advancement. With this convention, a cupellation progress Table 3 ﬁ of 0 represents the initial system (i.e. the lead bullion before the Summary of the re-assays. Bi and Ag content were analysed by ICP-SMS (HR-ICP- MS). start of the reaction), while a cupellation progress of 1 represents the ﬁnal system (i.e. silver button at the end of cupellation). Fire-assay Mass of lead Bi Ag Time Mass of silver Ag identiﬁcation bullion (g) content content (min) button (g) yield (ppm) (ppm) (%)a 3. Results Experimentation 1 (XP 1) Batch 1 In total, 28 ﬁre-assays were carried out. A silver button was XP1.1-1 20.72 130 7300 38 0.2564 169.5%b obtained for each of them. A summary of the experimental data is XP1.1-2 21.2 130 7300 36 0.1481 95.7% given in Table 3. XP1.1-3 22.94 130 7300 31 0.1598 95.4% XP1.1-4 16.74 130 7300 38 0.1186 97.1% 3.1. Macroscopic observation of the cupels after ﬁre-assays Batch 2 XP1.2-1 20.15 3000 10 000 35 0.1928 95.7% XP1.2-2 21.2 3000 10 000 40 0.2052 96.8% As evidenced on pictures presented in Fig. 2, an obvious differ- XP1.2-3 22.13 3000 10 000 37 0.2093 94.6% ence between the batches is the presence of a brown ring at the XP1.2-4 17.63 3000 10 000 30 0.1718 97.4% initial periphery of the lead bullion for all ﬁre-assays of XP1. As Batch 3 deduced from its location, the ring formed at the beginning of XP1.3-1 20.54 21 000 10 000 40 0.1912 93.1% ﬁ XP1.3-2 20.73 21 000 10 000 38 0.1927 93.0% cupellation. No ring is observed for re-assays of XP2, thus its XP1.3-3 21 21 000 10 000 36 0.2003 95.4% formation is clearly not linked to the Bi content and can rather be XP1.3-4 18.26 21 000 10 000 40 0.1520 83.2% attributed to the high Sb and Sn contents in lead bullions of XP1. Experimentation 2 (XP 2) The major colour difference between the batches is located right Batch 1 XP2.1-1 18.75 9900 10 100 64 0.1775 93.9% around the silver button where a quite distinctive brownish oxide XP2.1-2 21.14 9900 10 100 36 0.1986 93.2% surrounded by a dark green circle appears in XP1-3 and all batches XP2.1-3 22.35 9900 10 100 35 0.2135 94.8% from XP2. XP1-2 also shows a slight colour change to a yellow XP2.1-4 20.2 9900 10 100 30 0.1926 94.6% brownish tint around the silver button, yet not as marked as on the Batch 2 other cupels. This feature clearly indicates a change in the oxide XP2.2-1 20.23 19 400 10 200 33 0.1917 93.0% XP2.2-2 18.1 19 400 10 200 28 0.1695 91.9% composition that penetrated the cupels at the end of the process, XP2.2-3 21.71 19 400 10 200 30 0.2042 92.3% and concerns Bi rich batches. XP2.2-4 22.3 19 400 10 200 33 0.2154 94.8% Batch 3 3.2. Microscopic observation and chemical mapping with SEM-EDS XP2.3-1 22.34 38 600 10 000 34 0.2063 92.8% XP2.3-2 19.38 38 600 10 000 32 0.1772 91.9% XP2.3-3 19.7 38 600 10 000 32 0.1816 92.6% One cupel per batch of XP1 was crosscut in order to characterize XP2.3-4 23 38 600 10 000 37 0.2097 91.6% and observe the distribution of metal oxides through the cupels. Batch 4 The three cartographic views presented in Fig. 3 show that Pb XP2.4-1 19.46 78 100 10 200 35 0.1789 90.6% impregnated the entire cupels from the bottom to the top (i.e. from XP2.4-2 21.38 78 100 10 200 32 0.1972 90.9% ﬁ XP2.4-3 22.16 78 100 10 200 34 0.2052 91.2% the rst to the last litharge respectively). The distribution of the XP2.4-4 23.38 78 100 10 200 38 0.2099 88.5% impurities (Bi, Sb, Sn), rather similar for each batch, is highly a Yield ¼ Y ¼ ((m (Ag)button/m (Ag)initial))*100. dependent on the nature of the element: b Such yield indicates that cupellation was not completed, which is consistent with the absence of gas expulsion observed for this sample (no cauliﬂowering). This Sb and Sn are mainly located in the brown rings and at the run was disregarded in the results treatment. bottom of the cupels Bi is located at the top of the cupels, i.e. in the last litharge 3.4. Silver extraction yields
ﬁ 3.3. Concentration proﬁle of cupels using microprobe For each re-essay, the silver extraction yield (Y) was calculated as the ratio of the silver button mass to the initial mass of silver Three chemical proﬁles, presented in Fig. 4, were obtained from the bottom to the top of the cupels from XP1, vertically to the location of the Silver button (see Fig. 3). Ag and Bi exhibit a similar behaviour: their concentration is very low in most of the litharge, and at approx. À2000 mm depth, a noticeable increase is observed. Ag concentration proﬁles are similar for each cupellation, which is consistent with a constant Ag initial concentration in the initial lead bullion. Bi content increases in the last litharge (0 to À500 mm depth) according to its initial concentration in the lead bullion. In XP1.3, Bi content exceeds Pb content in the last litharge. Apart from this speciﬁc case, Pb content is rather constant and constitutes the major element of litharge. Consistently with the chemical mapping presented in Fig. 3, microprobe analysis indicated very low Sb and Sn contents in the last litharge (values are scattered around the detection limits of respectively 0.010 and 0.015 wt.%) and a much higher content in the ﬁrst litharge (notably above the quantiﬁcation limits of respectively ﬁ 0.10 and 0.15 wt.%). This con rms that most of Sb and Sn were Fig. 2. Macroscopic view of the cupels seen from above after the seven ﬁre-assays (one conﬁned in the brown ring. cupel per batch). Fig. 3. Optical view and elemental mapping (acquired by SEM-EDS) of cupels from experiments XP1-1-2, XP1-2-3 and XP1-3-1. present in the lead bullion (Table 3), assuming that silver buttons no clear correlation was found between the Bi content of the ﬁnal are composed of pure silver (see below “Chemical composition of silver button and that of the initial lead bullion. the silver button”). Yet, as illustrated in Fig. 6, despite a signiﬁcant standard devi- Silver extraction yields are reported in Fig. 5 versus the initial Bi ation in the Pb and Bi concentrations, a linear correlation between content of lead bullions. A linear decrease of the yield e from the Bi/Pb ratio in the silver button and the Bi content in the initial average 96.1% for XP1.1 (130 ppm Bi) to average 90.3% for XP2.4 lead bullion was evidenced for both experimental campaigns. (7.8 wt.% Bi) e is evidenced. 3.6. Thermochemical calculations
3.5. Chemical composition of the silver button The volatility of Bi element was evaluated as a preliminary calculation, in order to verify that Bi could be considered as a tracer. Analyses of the silver buttons by LA-ICP-MS (Table 4) reveal that At 1000 C, the vapour pressure of pure Bi is about 2$10À3 bar, while À6 they are mostly composed of pure silver (>99.9%). Pb and Bi are the the vapour pressure of pure Bi2O3 is 3$10 bar. These low values main impurities and other trace elements such as Sb and Sn are indicate that negligible evaporation of the Bi element occurs. It is almost totally absent with concentrations below 1 ppm. Pb con- thus considered that, during the cupellation process, there is no centration is scattered between 2 and 25 ppm, with an average loss of Bi in the atmosphere: either it stays in the button, or it value of 15 ppm independent of the initial Bi content. Bi presents oxidises in litharge. wider variations: it is logically absent for Bi poor batches XP1-1 Calculations related to cupellation reaction were performed for (0.5 ppm in average) and rises up to 10e30 ppm for XP1.2, XP1.3, the seven lead bullion compositions processed in XP1 and XP2 XP2.1 and XP2.2 and 100e200 ppm for XP2.3 and XP2.4. However, (Table 1). Since very similar trends were obtained regarding the individual behaviour of Sb, Sn, Pb, Bi and Ag, the results presented here are mostly focused on the case of XP1.2 (3000 ppm Bi, high Sn and Sb content) and XP2.2 (19 400 ppm Bi, low Sb and Sn content). The evolution of the composition of the metal phase vs. cupel- lation progress is given in Fig. 7. Two plots (Fig. 7, top) represent the mass of each element left in the metal phase related to its initial mass, during the whole cupellation reaction. As the oxidation of bismuth and silver mostly occurs at the end of the reaction, a focus depicts the evolution of the mass of Pb, Ag and Bi in the metal phase for cupellation progress over 0.8 (Fig. 7, bottom). The litharge phase composition is plotted in Fig. 8: the mass fraction of each element is indicated, and, again, a focus for cupellation progress over 0.8 is included. It can be noted that, for high Bi initial content (which is typically the case of XP2.2), litharge contains more Bi than Pb at the very end of the reaction (cupellation progress > 0.95). This composition is thus outside the range of the model hypothesis, which considers a main PbO phase with diluted components. The ﬁnal Pb content in the silver button was calculated between Fig. 5. Evolution of experimental silver extraction yield vs. Bi content in the initial lead 20 and 100 ppm, depending on the value of the calculation step (i.e. bullion for all batches (except XP1-1-1 and XP1-3-4).
Table 4 Average composition of experimental silver buttons analysed by LA-ICPeMS.
Reference Number of analyses Ag (%) Sn (ppm) Sb (ppm) Pb (ppm) Bi (ppm)
XP1-1 5 99.99 <1 nda 19 ± 10 0.5 ± 0.4 XP1-2 7 99.99 <1 nd 22 ± 10 11 ± 10 XP1-3 7 99.99 <1 nd 2 ± 2 9 ± 4 XP2-1 8 99.99 <1 <1 28 ± 7 27 ± 7 XP2-2 7 99.99 <1 nd 6 ± 4 24 ± 20 XP2-3 8 99.97 <1 <1 25 ± 27 209 ± 98 XP2-4 6 99.99 <1 nd 9 ± 10 70 ± 52
a Not detected (nd) values are likely under 0.1 ppm.
the amount of air added in the system at each step). Similarly, the ﬁnal Bi content in the silver button was highly dependent on the step value, while the Bi/Pb ratio was found much less sensitive to this calculation artefact. Fig. 9 shows the evolution of the Bi/Pb ratio in the metal phase for XP1-1, XP1-2, XP1-3 and XP2-2 during cupellation, together with the experimental ratio measured in the silver button. Finally, the calculation of the Ag and Bi contents in an “average” litharge (i.e. calculated for a cupellation progress of 0.4), depending on the initial Ag and Bi content in the lead bullion, is presented in Fig. 10.
Fig. 4. Microprobe vertical proﬁles of three cupels from XP1 (1-2, 2-1 and 3-1) for Pb, Fig. 6. Evolution of experimental Bi/Pb mass ratio in silver button vs. Bi content in the Ag and Bi elements. initial lead bullion. 4. Discussion reactions involving the lining taking place at the beginning of the cupellation. The following results are therefore valid for any kind of 4.1. Chemical elements behaviour during cupellation archaeological cupellation hearth material.
The combination of experimental results and modelling pro- vides a clear picture of the behaviour of each element during the 4.1.1. Behaviour of Sn and Sb cupellation process. The major element of the system, Pb, oxidises Calculations indicate that Sb and Sn elements oxidise at the during the whole process to form litharge, and the reaction stops beginning of the cupellation (Figs. 7 and 8). At the very beginning of e when only traces of Pb are left in the silver button. Experimental cupellation, the formation of a solid SnO2 Sb2O3 phase was data indicate a residual Pb concentration of 2e20 ppm in the silver computed in the case of XP1.2 and XP1.3, corresponding to Sn and button, while calculations lead to a higher concentration, in Sb-rich lead bullions. For all XP1 compositions, it was also shown 20e100 ppm range, in good accordance with the model of Swin- that, up to cupellation progress of about 0.2, litharge major bourne (Swinbourne et al., 2003). component was Sb (Fig. 8). These calculations are experimentally Sn, Sb and Bi also fully oxidise to litharge during the reaction. supported by the presence of rings on the outer rim of cupels from However, Sn and Sb oxidise at the beginning of cupellation (as a XP1 (Fig. 2), where Sb and Sn were located by SEM-EDS exploration dross and in the ﬁrst portions of litharge), while Bi oxidises mainly (Fig. 3). Theses rings are most probably composed of a mixture of e at the end of cupellation (in the last portions of litharge). A small SnO2 Sb2O3, lead antimonate (Pb2Sb2O7) and lead tin oxide e e e proportion of silver ﬁnally oxidises at the very end of cupellation. (Pb2SnO4), which are stable compounds in the Sb Sn Pb O sys- A discussion on the speciﬁc behaviour of each element is pre- tem likely to separate as dross on the surface of the metallic bath sented in this section. Former studies on archaeological cupels (Schnabel, 1898). This matches with studies published by Pernicka showed that cupellation hearth material does not affect the et al. (1998), indicating that lead antimonates were observed in ﬁ composition of the produced litharge nor the silver yield (see x 2.2). samples of archaeological litharges formed in the rst stages of Thus, changes in its composition seem quite unlikely to distort cupellation, with Sb contents up to 5 wt.% locally, near the surface radically neither the elemental behaviour of Bi nor the silver yield. of the litharge cake. The authors suspect this feature to be the Moreover, as silver losses and bismuth oxidation mainly occur at remainder of such dross that has not completely molten and was the end of the reaction they should not be greatly impacted by not properly skimmed off from the cupellation bath. Mass et al. (2002) also report that these Sb-rich litharges and dross might
Fig. 7. Computed metal phase composition vs. cupellation progress for two initial compositions of the lead bullion (XP1-2 and XP2-2). Top: evolution of the mass ratio m/minitial of each element during the whole reaction. Bottom: evolution of the metal composition (g for 100 g of lead bullion) for 0.8 < cupellation progress < 1. Fig. 8. Computed litharge phase composition (in mass fraction of elements) vs. cupellation progress for two initial compositions of the lead bullion (XP1-2 and XP2-2). Top: evolution of the litharge composition during the whole reaction. Bottom: evolution of the litharge composition for 0.8 < cupellation progress < 1. have been used in ancient yellow and green Roman glasses. Our antimony will form solid dross rather than stay in solution in the experiments conﬁrm that producing such lead antimoniate and litharge. Nevertheless, SEM-mapping and microprobe analyses of separating it from the cupellation bath was natural when pro- the experimental cupels testify that despite this behaviour a small cessing Sb-rich lead ores, due to dross formation in the early proportion of both elements is still present in the ﬁrst portions of cupellation stages. Such valorisation and trade of this by-product litharge and thus in lead recovered from litharge resmelting. should be looked for in future archaeological studies on regions with Sb-rich lead ores deposits. Regarding litharge composition, it seems clear that, even if present in large proportions in the processed alloy, tin and
Fig. 9. Calculation of Bi/Pb ratio evolution in the metal phase vs. cupellation progress Fig. 10. Calculation of Ag (left y-axis) and Bi (right y-axis) content in an average for four initial lead bullion compositions (XP1-1, XP1-2, XP1-3 and XP2-2). Comparison litharge (cupellation progress ¼ 0.4) depending on the initial Ag or Bi content in the to experimental Bi/Pb ratio in silver buttons of XP1. lead bullion. Estimating this proportion was however not possible with the all lead bullion compositions regardless of their Bi content. This is present data. likely to be due to the description of the litharge phase used in the Concerning the methodology of the present work and the fact model: litharge is considered as a PbO phase including dilute that Sb and Sn oxidise at the beginning of cupellation, the great amounts of Ag, Bi, Sb and Sn oxides. However, as shown by the difference regarding Sb and Sn contents in the initial alloys be- concentration proﬁle of XP1.3-1 (Fig. 4), the colour changes of cu- tween XP1 and XP 2 is believed to have no impact on Ag and Bi pels (Fig. 2) and the calculations (Fig. 8), the last portions of litharge behaviours at the end of the cupellation. in the case of high initial Bi contents are richer in Bi than in Pb. Thus, the model is not adapted for calculations at cupellation 4.1.2. Behaviour of Ag progress above 0.95e0.99, depending on the initial Bi content. The Silver losses (about 2e5 wt.%) as measured in low Bi-content most likely explanation is that the model does not take into account ﬁre-assays are due to silver oxidation at the end of cupellation. a possible ternary interaction in the PbOeBi2O3eAg2O system. Indeed, the concentration proﬁles in the cupels indicate a strong Indeed, even if Bi2O3 and PbO dissolve Ag2O roughly in the same increase of Ag content in the last portions of litharge (Fig. 4). proportion (about 5 wt.%), a PbOeBi2O3 mixture might enhance Accordingly, the present model shows that for lead bullions con- Ag2O solubility, and thus lead to an increase of Ag2O loss with taining 1 wt.% Ag, litharge should bear about 50e100 ppm Ag increasing Bi content. However, no thermochemical data was found during most of the reaction, while a content reaching up to a few to assess this assumption. Regarding material where bismuth is wt.% is expected in the last portions of litharge (Fig. 8), leading to a largely in excess, Berthier (1834) also registered enhanced silver silver reaction yield of about 96%. This result ﬁts with experiments loss and suggested that it mainly occurs by impregnation, as, ac- conducted at Pongibaud and quoted by Percy (1870) stating that Ag cording to him, bismuth oxide is more ﬂuid than lead oxide and content in litharge is quite constant throughout the ﬁrst stages of carries away more silver within the pores of the cupel. However, the process and reaches 4e8 g of silver in 100 kg of litharge (i.e. modern data rule out Berthier's hypothesis, since, at 1000 C, the 40e80 ppm) for lead initially bearing as much as 6000 ppm Ag. The viscosity of PbO is 0.003 Pa s (Oliver, 1965) while the viscosity of more recent work of Swinbourne et al. (2003), which focuses on Bi2O3 is 0.01 Pa s (Meshalkin and Kaplun, 2005). modern industrial cupellation process conﬁrms that silver losses in Regarding the produced silver, experimental data show (Fig. 6) litharge occur at the end of the reaction. Moreover, the present that the ﬁnal Bi/Pb ratio in the silver button is increasing with the thermochemical model demonstrates that the mean Ag content in initial Bi content, while no clear tendency could be drawn from the “average” litharge (i.e. for cupellation progress ¼ 0.4) is propor- ﬁnal Bi content vs. the initial Bi content. As evidenced in Fig. 9, tional to the Ag content in the initial lead bullion (Fig. 10), according combining calculation and experimental results, the Bi/Pb ratio in to the relation: Ag(ppm in litharge) ¼ 0.007 Ag(wt.% in lead bullion). This the metal phase is clearly dependent on the initial Bi content during matches with previous experimental work (Berthier, 1834; the whole process. Shephard and Dietriech, 1940) stating that in reproducible condi- Regarding litharge, the thermodynamic model shows that Bi tions silver loss is proportional to the initial Ag content. Available content in the ﬁrst portions of litharge (“average” litharge) is archaeological litharge analyses which could be compared with our directly proportional (by a factor of about 0.14) to the initial Bi data are however scarce in literature; ﬁrst because few smelting content in the lead bullion (Fig. 10). For example, in XP1.2 sites were excavated and second because litharge cakes were likely (3000 ppm Bi in lead bullion), litharge should contain an average of to be reduced into metallic lead whereas the last portions of silver- 300e400 ppm Bi. The chemical analyses of the cupels (Fig. 4) do rich litharge were reprocessed in order to recover the remaining however not allow to discuss about the Bi content of the ﬁrst silver. Litharge dated from the Bronze Age studied by Gale and Stos- portions of litharge (bottom of the cupel up to À2000 mm depth) Gale (1981) shows a Ag content usually below 50 ppm but reaching because of its low concentration, below the quantiﬁcation limit 200 ppm for a few samples. Syrian litharge dated from 3300 BC (about 800 ppm). Furthermore, comparison with published Bi-rich displays Ag content below 25 ppm for most samples but one litharge analysis is difﬁcult owing to their scarcity. reaching 3000 ppm (Pernicka et al., 1998). These archaeological values vary widely; nevertheless, based on the present work, they 4.2. Archaeological implications seem to indicate that the present archaeological artefacts are coming from different steps of the cupellation process: silver-rich These results provide new means for interpreting archaeological last portions of litharge (above 500 ppm) which could be retrea- remains linked to lead and silver production. They also shed light ted and silver-poor ﬁrst portions of litharge (below 100 ppm) which on technological choices made by the ancient metallurgists when could also be retreated or reduced to metallic lead. processing Bi-rich ores or lead bullions.
4.1.3. Behaviour of Bi and inﬂuence of Bi content 4.2.1. Silver materials Bismuth compounds are not volatile in the 900e1000 C tem- Both the model and the experimentations show that Bi does not perature range, as shown by thermochemical calculations. Ac- stay in the silver bullion and mainly oxidises at the end of cupel- cording to our experiments, Bi slightly oxidises at the beginning of lation. The amount of Bi remaining in the silver button relies the process and mostly at the end in the last portions of litharge therefore on the ﬁnal cupellation progress rather than on the initial alongside with Ag. This result matches with late 19th century Bi concentration of the lead bullion. This ﬁnal cupellation progress treatises such as Percy (1870) and Schnabel (1898) endorsed by depends on the type of process: whereas assaying tends to obtain more recent works (Shepard and Dietrich, 1940; Pernicka and pure silver, large-scale cupellation process does not. In order to Bachmann, 1983). Furthermore, our experimental data allow eval- avoid silver losses at the end of the process, large-scale cupellation uating the inﬂuence of the initial Bi concentration on the cupella- was usually conducted in several steps (Agricola, 1556; Biringuccio, tion process, especially regarding the evolution of the silver 1540; Ercker, 1580; Hawthorne and Smith, 1979). The operation was extraction yields. stopped several times (sometimes involving further addition of The decrease of the silver reaction yield with the increase of the lead) and led to the production of unreﬁned silver containing initial Bi content is clearly evidenced by experimental results varying amounts of lead and other impurities such as bismuth. (Fig. 5). The thermochemical model does however not account for Table 5 gives more details on the metal phase composition and this fact, since constant silver yield of about 96% was computed for its evolution near the end of the process as well as of the (Bi/Ag)/ (Bi/Ag)0 ratio according to our thermodynamic model. For an initial 10e30 times poorer in Bi than the initial lead bullion prior to the Bi concentration of 3000 ppm (XP 1.2), ﬁnal Bi contents up to 8 wt.% cupellation, i.e. 3e10% of the initial lead Bi content. can be expected in the silver depending on its reﬁnement, whereas This result has a direct consequence on the identiﬁcation means for 2 wt.% initial Bi (XP 2.2), unreﬁned silver containing up to of desilvered lead, which were so far mainly based on Ag content 30 wt.% Bi and silver containing as much as 7 wt.% Bi can be pro- only (Tylecote, 1986; Rehren and Prange, 1998; Asderaki and duced. High Bi contents up to several percent found in archaeo- Rehren, 2006). According to our study, among all chalcophile ele- logical unreﬁned silver (Craddock et al., 1985; Renzi et al., 2007) ments, alongside silver, bismuth seems best to provide a new mean seem to be in very good agreement with our data. to estimate whether lead was desilvered or not. This potential Regarding the evolution of Bi contents throughout the reaction, discrimination remains of course highly dependent on the experiments carried out by Pernicka and Bachmann (1983) state composition of the processed ores and the archaeological context. that the Bi/Ag ratio in the metal phase decreases by a ratio of about For example, all lead ingots from the roman period analysed by ﬁve to ten during cupellation. Our model shows that this order of Baron and Cochet (2003) would be coming from desilvered litharge magnitude is highly dependent on the reaction advancement as resmelting. Most of them indeed exhibit very low Bi concentrations well as on the initial Bi content. During cupellation, the (Bi/Ag)/(Bi/ (<15 ppm) associated with low Ag content (<70 ppm) typical for Ag)0 ratio changes from a relation of approximately four (1/0.3 for this kind of lead. Even three ingots bearing respectively 100, 140 XP 1.1) to twenty (1/0.05 for XP 2.2) (Table 5), and is even likely to and 220 ppm of silver could be compatible with this hypothesis as be much higher when quite “pure” silver (>95%) is to be obtained, no relevant difference in their Bi content could be highlighted. largely amplifying the results proposed by Pernicka and Bachmann Such reﬂexion led on much larger sets of lead artefacts might, in (1983). Large portions of Bi seem therefore in any case irremediably the near future, highlight the importance at a given time and place lost to litharge in the end of the process (see x 4.2.3). of simple fusion and desilvered lead. Nonetheless, as the Bi/Pb ratio in the metal phase is clearly dependent on the initial Bi content throughout the whole reaction 4.2.3. Processing Bi-rich ores: a metallurgical challenge? (Fig. 9), a more precise estimation of the initial Bi content of the Results on silver loss during the cupellation of Bi rich silver lead lead bullion can be proposed using Fig. 6. The use of this ratio is bullions question as well the technical aspects of processing very likely to allow distinguishing between different silverelead stocks rich Bi ores for silver production. One can suspect that metallurgists regardless of the reaction advancement much rather than pure Bi avoided such silver losses of 5e10% due to the presence of Bi during concentrations. It should however not be forgotten that in many cupellation. For example, silver loss can be spared when processing archaeological objects, further lead or copper addition, mixing of CueAg ores by the addition of an excess of lead, which prevents different metal sources in mints as well as frequent remelting and silver dilution in Cu2O(Bayley and Eckstein, 2006). However, as reminting of ancient coins might very much erase this signature. Bi2O3 and PbO dissolve Ag2O roughly in the same proportion, the However, in a production context, computing this ratio provides present hypothesis favours a PbOeBi2O3 interaction enhancing estimations of the initial Bi concentration of the lead bullion pro- silver dilution. Lead addition might therefore not reduce silver cessed by cupellation and therefore on the materials which were losses as for the case of CueAg ores. Such silver loss in litharge, treated by ancient metallurgists and their recipes. alongside a fraction of bismuth, would seem here ineluctable when quite pure silver is to be obtained. These last silver and Bi rich portions of litharge were certainly retreated to improve the silver 4.2.2. Lead materials yield. Another challenge is to identify these technological decisions Further reﬂection on lead artefacts is linked to the hypothesis in archaeological remains. Very rich lead and bismuth material also that lead coming from litharge resmelting would reﬂect the containing silver from the Tartessian site of Penalosa~ in Spain (Hunt composition of an average litharge. This last comparison between Ortiz, 2003) could indeed match with the retreatment of such Bi- resmelted lead and litharge compositions is however subject to rich last portions of litharge and testify of the metallurgical caution, as metallic lead was not produced in our experiments. It is choices improving the efﬁciency of the process. These archaeo- therefore impossible so far to assert whether litharge resmelting logical examples are however scarce so far and future archaeolog- radically modiﬁes the Bi content in lead materials or not. This ical work should stress on this point to understand the speciﬁc point would require further experiments and technological decisions taken by the ancient metallurgists for investigations. processing this kind of ore and improve its efﬁciency. Comparison Nevertheless, assuming this hypothesis, Bi content in archaeo- between the composition of both Bi-rich ore mining sources and logical lead materials would mainly be a tracer of metallurgical lead and silver archaeological artefacts produced in the same re- processes as it should represent roughly 10e15% of its content in gions should be investigated to highlight the frequency but also the the initial lead bullion before cupellation (Fig. 10). This ratio is technical aspects of processing such Bi-rich ores. Further archaeo- endorsed by experiments conducted by L'Heritier and Tereygeol logical investigations and ﬁne analysis of silver and lead artefacts (2010) who claim that lead coming from litharge resmelting is such as undergoing in the French site of Castel-Minier will be
Table 5 required to elucidate these interrogations.
Evolution of Bi and Ag contents and of the (Bi/Ag)/(Bi/Ag)0 ratio in the metal phase near the end of the cupellation process according to the thermodynamic model. 5. Conclusions
Cupellation XP 1.2 XP 2.2 progress This interdisciplinary approach focused on the behaviour of Bi, Ag (%) Bi (%) (Bi/Ag)/(Bi/ Ag (%) Bi (%) (Bi/Ag)/(Bi/ Sb and Sn during the cupellation process. Sb and Sn are carried Ag)0 Ag)0 away in the early stage of cupellation, and partially form solid 0.95 16 4 0.72 24 24 0.55 compounds, but noticeable amounts of these elements are still 0.96 22 5 0.7 29 27 0.5 0.97 31 6 0.65 38 31 0.4 likely to be present in the produced litharge cake. Bi is not volatile 0.975 36 6 0.6 47 31 0.35 and distributes between the litharge and metal phase with an 0.98 44 7 0.55 60 26 0.25 average ratio of one to ten during the ﬁrst 80% of the reaction. It 0.985 57 8 0.5 77 16 0.1 mostly oxidises at the end of the reaction and is ﬁnally present in 0.99 80 7 0.3 92 7 0.05 very small proportions in the resulting silver button in assaying conditions. Moreover, the presence of Bi in the processed alloy has a Betterton, J.O., Lebedeff, Y., 1936. Debismuthing lead with alkaline earth metals. e detrimental effect on the silver yield. Trans. Am. Inst. Min. Metall. Eng. 121, 205 225. Biringuccio, V., 1540. De la Pirotechnia. The Pirotechnia of Vannoccio Biringuccio, the Bi can be considered as an ore source tracer for silver material Classic Sixteenth-Century Treatise on Metals and Metallurgy (C.S. Smith, M.T. using the Bi/Pb ratio. Thermodynamic calculations assessed by Gnudi, Trans.), 1990. Dover Publications, New York. € experimental data offer predictive tools to estimate the initial Bode, M., 2008. Archaometallurgische Untersuchungen zur Blei-/Silbergewinnung im Germanien der frühen Romischen€ Kaiserzeit. Dissertation 2008, Münster, quantities of Bi present in the lead bullions as well as the resulting Online. http://nbn-resolving.de/urn:nbn:de:hbz:6-22579580819. Bi and Ag passing in litharge. These data will not be so useful for Chaudet, L.J., 1818. Sur la volatilite du bismuth. Ann. Chim. Phys. 9, 397e400. ﬁnished objects such as coins, in which the elemental signature is Cincotti, A., Massidda, L., Sanna, U., 2003. Chemical and isotope characterization of lead ﬁnds at the Santa Barbara nuraghe (Bauladu, Sardinia). J. Cult. Herit. 4, erased due to metal mixing and remelting, but could be used on 263e268. metallurgical production sites, to study ore selection, recipes and Cowell, M.R., Lowick, N.M., 1988. Silver from the panjhir mines. In: Oddy, W.A. (Ed.), technological choices as well as efﬁciency of the metallurgical Metallurgy in Numismatics, 2, pp. 65e74. London. Craddock, P.T., Freestone, I.C., Gale, N.H., Meeks, N.D., Rothenberg, B., Tite, M.S., processes. 1985. The investigation of a small heap of silver smelting debris from Rio Tinto, Interpretations are more complex for metallic lead based arte- Spain. In: Craddock, P.T., Hughes, M.J. (Eds.), Furnaces and Smelting Technology facts which are likely to come from unreﬁned or desilvered lead, or in Antiquity, British Museum Occasional Paper 48, pp. 199e217. London. mixed during recycling. However, should no important remobili- Cuzange, L., Texier, A., 2000. Caracterisation de plombs anciens de vitraux. In: Corpus Vitrearum Newsletter, n 47, pp. 43e51. sation of trace element between litharge and resmelted lead be Defonte, M., 1964. Les composes intermetalliques deﬁnis et leurs applications au assessed, Bi would also be a tracer of sources and metallurgical debismuthage du plomb. Memoire du Conservatoire National des Arts et processes for archaeological leads. Low Bi contents could be Metiers, p. 40. Diop, I., David, N., Fiorani, J.M., Podor, R., Vilasi, M., 2009. Experimental in- explained by the use of Bi-poor lead ores as well as by their tech- vestigations and thermodynamic description of the PbO-Bi2O3 system. J. Chem. nological origin, i.e. desilvered lead coming from cupellation. Thermodyn. 41, 420e432. Ercker, L., 1580. Lazarus Ercker's Treatise on Ores and Assaying (A.G. Sisco, C.S. Smith, Trans.), 1951. University of Chicago Press, Chicago. Acknowledgements Evers, D., 1949. Debismuthage par le proced e de Kroll-Betterton. Erzmetall 9. Forel, B., Monna, F., Petit, C., Bruguier, O., Losno, R., Fluck, P., Begeot, C., Richard, H., Bichet, V., Chateau,^ C., 2010. Historical mining and smelting in the Vosges All analyses and samples preparation have been performed in Mountains (France) recorded in two ombrotrophic peat bogs. J. Geochem. CNRS laboratories, in France (except elemental analyses of the Explor. 107, 9e20. home made lead alloys). Thus, we would like to thank the team of Gale, N.H., Stos-Gale, Z.A., 1981. Cycladic lead and silver metallurgy. Annu. Br. Sch. e the rocks workshop located in GET laboratory (Fabienne de Par- Athens 76, 169 224. Grandjean de Fouchy, J.-P., 1757. Sur le bismuth, Histoire de l'Academie royale des seval, Jean-François Mena and Ludovic Menjot). Many thanks to sciences, annee 1753, pp. 190e194. Section « Histoire ». Philippe de Parseval, Sophie Gouy and Thierry Aigouy from the Hawthorne, J.G., Smith, C.S., 1979. Theophilus: on Divers Arts. Dover, New, York. Microanalyses Service of the GET laboratory also. Special thanks to Hunt Ortiz, M., 2003. Prehistoric Mining and Metallurgy in South West Iberian Peninsula. In: British Archaeological Reports, International Series, vol. 1188. Guillaume Sarah and Maryse Blet-Lemarquand for their help with Archaeopress, Oxford. silver button analyses with the LA-ICP-MS located in IRAMAT lab- Kopyto, M., Przybylo, W., Onderka, B., Fitzner, K., 2009. Thermodynamic properties oratory. All experiments were conducted on the national experi- of Sb2O3-SiO2 and PbO-Sb2O3-SiO2 liquid solutions. Arch. Metall. Mater. 54 (3), 811e822. mental archaeology platform located in Melle (France). We would Kroll, W., 1922. Separati on dans les solutions metalliques. Met. Erz 19, 317e324. also like to thank warmly Mr. Bied-Charreton and Mr. Bertrand Kroll, W., 1938. Progres dans la separation des metaux. Met. Erz 35, 252e254, Dusanter (ERAMET Group) for their assistance to bibliographical 286e288. Kuleff, I., Iliev, I., Pernicka, E., Gergova, D., 2006. Chemical and lead isotope com- access on archives on industrial processes of the 19th and 20th positions of lead artefacts from ancient Thracia (Bulgaria). J. Cult. Herit. 7, centuries. 244e256. Kuleff, I., Djingova, R., Alexandrova, A., Vakova, V., Amov, B., 1995. INAA, AAS, and lead isotope analysis of ancient lead anchors from the black sea. J. Radioanal. References Nucl. Chem. 196 (1), 65e76. L'Heritier, M., Tereygeol, F., 2010. From copper to silver: understanding the saiger- Agricola, G., 1556. De re metallica (H.C. Hoover, L.H. Hoover, Trans.), 1950. Dover prozess through experimental liquation and drying. Hist. Metall. 44 (2), Publications, New York. 136e152. Anguilano, L., Rehren, T., Müller, W., Rothenberg, B., 2010. The importance of lead in Lu, D.-K., Jin, Z.-N., Jiang, K.-X., 2011. Fine debismuthizing with calcium, magnesium the silver production at Riotinto (Spain). ArcheoSci. Rev. archeom. 34, 269e276. and antimony. Trans. Nonferrous Metals Soc. China 21, 2311e2316. Asderaki, E., Rehren, T., 2006. The lead metal from two Hellenistic towns in east Mac Kerrell, H., Stevenson, R.B.K., 1972. Some analyses of Anglo-Saxon and associ- central Greece. In: Perez-Arantegui, J. (Ed.), Proceedings of the 34th Interna- ated Oriental Silver Coinage. In: Hall, E.T., Metcalf, D.M. (Eds.), Methods of tional Symposium on Archaeometry, Zaragoza, 3e7 May 2004. Institucion Chemical and Metallurgical Investigation of Ancient Coinage, 8. RNS Special Fernando el Catolico (C.S.I.C.), Zaragoza, pp. 131e136. http://www.dpz.es/ifc/ Publication, London, pp. 195e209. libros/ebook2621.pdf. Martinon-Torres, M., Rehren, T., Thomas, N., Mongiatti, A., 2009. Identifying mate- Assal, J., Hallstedt, B., Gauckler, L.J., 1999. Experimental phase diagram study and rials, recipes and choices: some suggestions for the study of archaeological thermodynamic optimization of the Ag-Bi-O system. J. Am. Ceram. Soc. 82 (3), cupels. In: Archaeometallurgy in Europe 2007. Selected Papers, of the 2nd In- 711e715. ternational Conference 17.e21. June 2007 in Aquileia. AIM, Milano, Atzeni, C., Cincotti, A., Massida, L., Sanna, U., 2003. Experimental lead “old metal- pp. 435e445. lurgy”. In: Archaeometallurgy in Europe, Milan, pp. 107e115. Martinon-Torres, M., Rehren, T., Thomas, N., Mongiatti, A., 2008. Some problems Bale, C.W., Chartrand, P., Decterov, S.A., Eriksson, G., Hack, H., Ben Mahfoud, R., and potentials of the study of cupellation remains: the case of post-medieval Melançon, J., Pelton, A.D., Petersen, S., 2002. FactSage thermochemical software Montbeliard, France. ArcheoSci. Rev. archeom. 32, 59e70. and databases. Calphad J. 62, 189e228, 2002. Mass, J.L., Wypyski, M.T., Stone, R.E., 2002. Malkata and light glassmaking tech- Baron, S., Cochet, A., 2003. Etude d'un lot de lingots de plomb antiques des Saintes- nologies: towards a speciﬁc link between second millennium BC metallurgists Maries-de-la-Mer. Segr egations et analyses chimiques el ementaires. La Rev. and glassmakers. Archaeometry 44 (1), 67e82. archeom. 147e163. Matthey, E., 1887. Contributions to the metallurgy of Bismuth. Proc. R. Soc. Lond. 42, Baron, S., Mahe-Le-Carlier , C., Carignan, J., Ploquin, A., 2009. Archaeological 89e94. reconstruction of medieval lead production: implications for ancient metal Meshalkin, A.B., Kaplun, A.B., 2005. Melt viscosity of binary system Bi2O3-GeO2. provenance studies and paleopollution tracing by Pb isotopes. Appl. Geochem. J. Cryst. Growth 275, 905e908. 24, 2093e2101. Ng, K., Siviour, N.G., 1994. A process for debismuthizing Lead with magnesium,. Bayley, J., Eckstein, K., 2006. Roman and medieval litharge cakes: structure and Metall. Mater. Trans. B 25b, 379e384. composition. In: Perez-Arantegui, J. (Ed.), Proceedings of the 34th International Oliver, C.B., 1965. Viscosity of some molten lead compounds. J. Electrochem. Soc. Symposium on Archaeometry, Zaragoza, 3e7 May 2004. Institucion Fernando el 112, 629e631. Catolico (C.S.I.C.), Zaragoza, pp. 145e153. Percy, J., 1870. The Metallurgy of Lead, Including Desilverisation and Cupellation Berthier, P., 1834. Traite des essais par la voie seche ou des propriet es, de la (London). € composition et de l'essai des substances, metalliques et des combustibles, Tome Pernicka, E., Bachmann, H.G., 1983. Archaometallurgische Untersuchungen zur 2. Paris. antiken Silbergewinnung in Laurion. Erzmetall 36, 592e597. Pernicka, E., Rehren, T., Schmitt-Strecker, S., 1998. Late Uruk silver production by Schnabel, C., 1898. Handbook of Metallurgy (H. Louis, Trans.). In: Copper, Lead, cupellation at Habuba Kabira, Syria. Der Anschnitt Beih. 8, 123e134. Silver, Gold (London), vol. I, p. 876. Pott, J.H., 1738. Exercitationes Chymicae. J. A. Rüdiger, Berolini. Shao, Z.B., Liu, K.R., Liu, L.Q., Liu, H.K., Dou, S.X., 1993. Equilibrium phase diagrams in Ramachandra Rao, S., 2006. Resource Recovery and Recycling from Metallurgical the systems PbO-Ag and CuO-Ag. J. Am. Ceram. Soc. 76 (10), 2663e2664. Wastes. In: Waste Management Series, vol. 7. Elsevier, p. 200. Shepard, O.C., Dietrich, W.F., 1940. Fire Assaying. New York, 277 pp. Raub, C.J., 1995. The metallurgy of gold and silver in prehistoric times. In: Suhling, L., 1976. Der Saïgerhüttenprozess, die Technologie des Kupferseigerns nach Morteani, G., Northover, J.P. (Eds.), Prehistoric Gold in Europe: Mines, Metal- dem frühen metalurgischen Schriftum (Stuttgart). lurgy and Manufacture, pp. 243e259. Dordrecht. Suhling, L., 1994. Die Technologie des Kupferseigerns in Zentraleuropa im 15. und Rehren, T., 1998. Kontext und Analyse der Aschkupellen von Oberstockstall. In: von 16. Jahrhundert e technische, okonomische€ und politische Aspekte. In: Osten, S. (Ed.), Das Alchemistenlaboratorium von Oberstockstall, Ein Fund- Benoit, P., Bideau, A. (Eds.), Mines et metallurgie, pp. 97e106. Lyon. komplex des 16. Jahrunderts aus Niederosterreich.€ Universitatverlag€ Wagner, Swinbourne, D.R., Yan, S., Hoang, G., Higgins, D., 2003. Thermodynamic modelling Innsbruck, pp. 333e348. of cupellation: activity of AgO0.5 in molten PbO at 1000 C. Trans. Inst. Min. Rehren, T., Prange, M., 1998. Lead metal and patina: a comparison. Der Anschnitt Metall. Sect. C Mineral Process. Extr. Metall. 112, 69e74. Beih. 8, 183e196. Tereygeol, F., Thomas, N., 2003. La coupellation des alliages cuivre e argent: Renzi, M., Hauptmann, A., Rovira, S., et al., 2007. Phoenician metallurgical pro- Approches experimentales de l'essai d'argent par voie seche. La Rev. archeom. duction at SE-Spain. In: Proceedings of the 2nd International Conference 27, 171e181. Archaeometallurgy in Europe, 2007. Grado-Aquileia [CD-ROM]. Tylecote, R.F., 1976. A History of Metallurgy. Metals Society, London, p. 182. Sarah, G., 2012. An analysis of early medieval silver coins: towards a better un- Tylecote, R.F., 1986. The Prehistory of Metallurgy in the British Isles. Maney Pub- derstanding of the trading role of the Adriatic emporia? In: Gelichi, S. (Ed.), lishing, London, p. 257. From One Sea to Another. Trading Places in the European and Mediterranean Ueda, S., Katsube, R., Yamaguchi, K., 2009. Distributions of Sn, Sb and Bi between Early Middle Ages (Comacchio), pp. 339e353. Ag-Pb alloy and PbO based melt at 1273 K, Materials Transactions. Jpn. Inst. Sarah, G., Bompaire, M., McCormick, M., Rovelli, A., Guerrot, C., 2008. Analyses Metals 50 (7), 1820e1823. el ementaires de monnaies de Charlemagne et Louis le Pieux du Cabinet des Ueda, S., Kumagai, T., Yamaguchi, K., 2005. Thermodynamic study on the Ag-Pb-O Medailles : l'Italie carolingienne et Venise. Rev. Numis. 164, 355e406. system at 1273 K, Materials Transactions. Jpn. Inst. Metals 46 (8), 1861e1864. Sarah, G., Gratuze, B., Barrandon, J.-N., 2007. Application of laser ablation induc- Zaharescu, M., Mihaiu, S., Zuca, S., Matiasovsky, K., 1991. Contribution to the study of tively coupled plasma mass spectrometry (LA-ICP-MS) for the investigation of SnO2 based ceramics, Part I: high temperature interactions of tin(IV) oxide with ancient silver coins. J. Anal. Atomic Spectrom. 22, 1163e1167. antimony(III) oxide and copper(II) oxide. J. Mater. Sci. 26, 1666e1672.